#------------------------------------------------------------------------------
#$Date: 2021-06-18 10:24:44 +0300 (Fri, 18 Jun 2021) $
#$Revision: 266557 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/35/1563561.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1563561
loop_
_publ_author_name
'Yang, Tao'
'Sun, Junliang'
'Croft, Mark'
'Nowik, Israel'
'Ignatov, Alexander'
'Cong, Rihong'
'Greenblatt, Martha'
_publ_section_title
;
 Ca4Fe3−xMnxO8−\dCl2: A new n=3 Ruddlesden--Popper
 oxychloride
;
_journal_issue                   6
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              1215
_journal_page_last               1220
_journal_paper_doi               10.1016/j.jssc.2010.03.019
_journal_volume                  183
_journal_year                    2010
_chemical_formula_sum            'Ca8 Cl4 Fe2.58 Mn3.42 O16'
_chemical_formula_weight         1050.43
_space_group_IT_number           139
_space_group_name_Hall           '-I 4 2'
_space_group_name_H-M_alt        'I 4/m m m'
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_H-M   'I 4/m m m'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            1
_cell_length_a                   3.7960(5)
_cell_length_b                   3.7960(5)
_cell_length_c                   30.846(6)
_cell_measurement_reflns_used    3871
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      35.5870
_cell_measurement_theta_min      3.9485
_cell_volume                     444.48(12)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.982
_diffrn_measured_fraction_theta_max 0.982
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0355
_diffrn_reflns_av_sigmaI/netI    0.0145
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       49
_diffrn_reflns_limit_l_min       -49
_diffrn_reflns_number            8035
_diffrn_reflns_theta_full        35.72
_diffrn_reflns_theta_max         35.72
_diffrn_reflns_theta_min         3.96
_exptl_absorpt_coefficient_mu    7.398
_exptl_absorpt_correction_T_max  0.9003
_exptl_absorpt_correction_T_min  0.5891
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details
;
CrysAlis RED, Oxford Diffraction Ltd.,
Version 1.171.32.15 (release 10-01-2008 CrysAlis171 .NET)
(compiled Jan 10 2008,16:37:18)
Numerical absorption correction based on gaussian integration over
			a multifaceted crystal model
;
_exptl_crystal_density_diffrn    3.924
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             509
_exptl_crystal_size_max          0.08
_exptl_crystal_size_mid          0.07
_exptl_crystal_size_min          0.01
_refine_diff_density_max         1.095
_refine_diff_density_min         -2.160
_refine_diff_density_rms         0.222
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.986
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     36
_refine_ls_number_reflns         372
_refine_ls_number_restraints     14
_refine_ls_restrained_S_all      0.986
_refine_ls_R_factor_all          0.0466
_refine_ls_R_factor_gt           0.0364
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0536P)²+4.4433P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0928
_refine_ls_wR_factor_ref         0.0968
_reflns_number_gt                304
_reflns_number_total             372
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            JSSC-2010-183-1215.cif
_cod_data_source_block           Ca8Cl4Fe2.58Mn3.42O16
_cod_original_sg_symbol_H-M      I4/mmm
_cod_database_code               1563561
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-y, x, z'
'y, -x, z'
'x, -y, z'
'-x, y, z'
'-y, -x, z'
'y, x, z'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-y+1/2, x+1/2, z+1/2'
'y+1/2, -x+1/2, z+1/2'
'x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z+1/2'
'-y+1/2, -x+1/2, z+1/2'
'y+1/2, x+1/2, z+1/2'
'-x, -y, -z'
'x, y, -z'
'y, -x, -z'
'-y, x, -z'
'-x, y, -z'
'x, -y, -z'
'y, x, -z'
'-y, -x, -z'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z+1/2'
'y+1/2, -x+1/2, -z+1/2'
'-y+1/2, x+1/2, -z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'y+1/2, x+1/2, -z+1/2'
'-y+1/2, -x+1/2, -z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mn1 Mn 0.5000 0.5000 0.0000 0.0071(3) Uani 0.57 16 d SP . .
Fe1 Fe 0.5000 0.5000 0.0000 0.0071(3) Uani 0.43 16 d SP . .
Mn2 Mn 0.5000 0.5000 0.87856(3) 0.0095(2) Uani 0.57 8 d SP . .
Fe2 Fe 0.5000 0.5000 0.87856(3) 0.0095(2) Uani 0.43 8 d SP . .
Ca1 Ca 0.0000 0.0000 0.94094(7) 0.0269(4) Uani 1 8 d S . .
Ca2 Ca 0.0000 0.0000 0.17920(5) 0.0155(3) Uani 1 8 d S . .
Cl1 Cl 0.5000 0.5000 0.21653(6) 0.0250(4) Uani 1 8 d S . .
O1A O 0.5000 0.0000 0.0114(5) 0.024(7) Uani 0.21(4) 4 d SPU . .
O1B O 0.593(3) 0.0000 0.0000 0.019(5) Uani 0.29(4) 4 d SPU . .
O2 O 0.078(5) 0.0000 0.4390(2) 0.024(5) Uani 0.25 2 d SP . .
O3 O 0.5000 0.0000 0.13097(15) 0.0264(9) Uani 1 4 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O2 Mn1 O2 167.4(7) 10_554 28
O2 Mn1 O2 12.6(7) 10_554 12_554
O2 Mn1 O2 180.00(7) 28 12_554
O2 Mn1 O2 180.00(7) 10_554 26
O2 Mn1 O2 12.6(7) 28 26
O2 Mn1 O2 167.4(7) 12_554 26
O2 Mn1 O2 162.2(10) 10_554 25
O2 Mn1 O2 12.6(7) 28 25
O2 Mn1 O2 167.4(7) 12_554 25
O2 Mn1 O2 17.8(10) 26 25
O2 Mn1 O2 167.4(7) 10_554 27
O2 Mn1 O2 17.8(10) 28 27
O2 Mn1 O2 162.2(10) 12_554 27
O2 Mn1 O2 12.6(7) 26 27
O2 Mn1 O2 12.6(7) 25 27
O2 Mn1 O2 12.6(7) 10_554 11_554
O2 Mn1 O2 162.2(10) 28 11_554
O2 Mn1 O2 17.8(10) 12_554 11_554
O2 Mn1 O2 167.4(7) 26 11_554
O2 Mn1 O2 167.4(7) 25 11_554
O2 Mn1 O2 180.00(7) 27 11_554
O2 Mn1 O2 17.8(10) 10_554 9_554
O2 Mn1 O2 167.4(7) 28 9_554
O2 Mn1 O2 12.6(7) 12_554 9_554
O2 Mn1 O2 162.2(10) 26 9_554
O2 Mn1 O2 180.00(7) 25 9_554
O2 Mn1 O2 167.4(7) 27 9_554
O2 Mn1 O2 12.6(7) 11_554 9_554
O2 Mn1 O1B 81.2(5) 10_554 19_565
O2 Mn1 O1B 91.61(11) 28 19_565
O2 Mn1 O1B 88.39(11) 12_554 19_565
O2 Mn1 O1B 98.8(5) 26 19_565
O2 Mn1 O1B 81.2(5) 25 19_565
O2 Mn1 O1B 88.39(11) 27 19_565
O2 Mn1 O1B 91.61(11) 11_554 19_565
O2 Mn1 O1B 98.8(5) 9_554 19_565
O2 Mn1 O1B 98.8(5) 10_554 3_655
O2 Mn1 O1B 88.39(11) 28 3_655
O2 Mn1 O1B 91.61(11) 12_554 3_655
O2 Mn1 O1B 81.2(5) 26 3_655
O2 Mn1 O1B 98.8(5) 25 3_655
O2 Mn1 O1B 91.61(11) 27 3_655
O2 Mn1 O1B 88.39(11) 11_554 3_655
O2 Mn1 O1B 81.2(5) 9_554 3_655
O1B Mn1 O1B 180.0 19_565 3_655
O2 Mn1 O1B 88.39(11) 10_554 17_655
O2 Mn1 O1B 98.8(5) 28 17_655
O2 Mn1 O1B 81.2(5) 12_554 17_655
O2 Mn1 O1B 91.61(11) 26 17_655
O2 Mn1 O1B 88.39(11) 25 17_655
O2 Mn1 O1B 81.2(5) 27 17_655
O2 Mn1 O1B 98.8(5) 11_554 17_655
O2 Mn1 O1B 91.61(11) 9_554 17_655
O1B Mn1 O1B 69.0(7) 19_565 17_655
O1B Mn1 O1B 111.0(7) 3_655 17_655
O2 Mn1 O1B 91.61(11) 10_554 1_565
O2 Mn1 O1B 81.2(5) 28 1_565
O2 Mn1 O1B 98.8(5) 12_554 1_565
O2 Mn1 O1B 88.39(11) 26 1_565
O2 Mn1 O1B 91.61(11) 25 1_565
O2 Mn1 O1B 98.8(5) 27 1_565
O2 Mn1 O1B 81.2(5) 11_554 1_565
O2 Mn1 O1B 88.39(11) 9_554 1_565
O1B Mn1 O1B 111.0(7) 19_565 1_565
O1B Mn1 O1B 69.0(7) 3_655 1_565
O1B Mn1 O1B 180.000(1) 17_655 1_565
O2 Fe1 O2 167.4(7) 10_554 28
O2 Fe1 O2 12.6(7) 10_554 12_554
O2 Fe1 O2 180.00(7) 28 12_554
O2 Fe1 O2 180.00(7) 10_554 26
O2 Fe1 O2 12.6(7) 28 26
O2 Fe1 O2 167.4(7) 12_554 26
O2 Fe1 O2 162.2(10) 10_554 25
O2 Fe1 O2 12.6(7) 28 25
O2 Fe1 O2 167.4(7) 12_554 25
O2 Fe1 O2 17.8(10) 26 25
O2 Fe1 O2 167.4(7) 10_554 27
O2 Fe1 O2 17.8(10) 28 27
O2 Fe1 O2 162.2(10) 12_554 27
O2 Fe1 O2 12.6(7) 26 27
O2 Fe1 O2 12.6(7) 25 27
O2 Fe1 O2 12.6(7) 10_554 11_554
O2 Fe1 O2 162.2(10) 28 11_554
O2 Fe1 O2 17.8(10) 12_554 11_554
O2 Fe1 O2 167.4(7) 26 11_554
O2 Fe1 O2 167.4(7) 25 11_554
O2 Fe1 O2 180.00(7) 27 11_554
O2 Fe1 O2 17.8(10) 10_554 9_554
O2 Fe1 O2 167.4(7) 28 9_554
O2 Fe1 O2 12.6(7) 12_554 9_554
O2 Fe1 O2 162.2(10) 26 9_554
O2 Fe1 O2 180.00(7) 25 9_554
O2 Fe1 O2 167.4(7) 27 9_554
O2 Fe1 O2 12.6(7) 11_554 9_554
O2 Fe1 O1B 81.2(5) 10_554 19_565
O2 Fe1 O1B 91.61(11) 28 19_565
O2 Fe1 O1B 88.39(11) 12_554 19_565
O2 Fe1 O1B 98.8(5) 26 19_565
O2 Fe1 O1B 81.2(5) 25 19_565
O2 Fe1 O1B 88.39(11) 27 19_565
O2 Fe1 O1B 91.61(11) 11_554 19_565
O2 Fe1 O1B 98.8(5) 9_554 19_565
O2 Fe1 O1B 98.8(5) 10_554 3_655
O2 Fe1 O1B 88.39(11) 28 3_655
O2 Fe1 O1B 91.61(11) 12_554 3_655
O2 Fe1 O1B 81.2(5) 26 3_655
O2 Fe1 O1B 98.8(5) 25 3_655
O2 Fe1 O1B 91.61(11) 27 3_655
O2 Fe1 O1B 88.39(11) 11_554 3_655
O2 Fe1 O1B 81.2(5) 9_554 3_655
O1B Fe1 O1B 180.0 19_565 3_655
O2 Fe1 O1B 88.39(11) 10_554 17_655
O2 Fe1 O1B 98.8(5) 28 17_655
O2 Fe1 O1B 81.2(5) 12_554 17_655
O2 Fe1 O1B 91.61(11) 26 17_655
O2 Fe1 O1B 88.39(11) 25 17_655
O2 Fe1 O1B 81.2(5) 27 17_655
O2 Fe1 O1B 98.8(5) 11_554 17_655
O2 Fe1 O1B 91.61(11) 9_554 17_655
O1B Fe1 O1B 69.0(7) 19_565 17_655
O1B Fe1 O1B 111.0(7) 3_655 17_655
O2 Fe1 O1B 91.61(11) 10_554 1_565
O2 Fe1 O1B 81.2(5) 28 1_565
O2 Fe1 O1B 98.8(5) 12_554 1_565
O2 Fe1 O1B 88.39(11) 26 1_565
O2 Fe1 O1B 91.61(11) 25 1_565
O2 Fe1 O1B 98.8(5) 27 1_565
O2 Fe1 O1B 81.2(5) 11_554 1_565
O2 Fe1 O1B 88.39(11) 9_554 1_565
O1B Fe1 O1B 111.0(7) 19_565 1_565
O1B Fe1 O1B 69.0(7) 3_655 1_565
O1B Fe1 O1B 180.000(1) 17_655 1_565
O2 Mn2 O2 12.7(7) 11 9
O2 Mn2 O2 12.7(7) 11 10
O2 Mn2 O2 18.0(10) 9 10
O2 Mn2 O2 18.0(10) 11 12
O2 Mn2 O2 12.7(7) 9 12
O2 Mn2 O2 12.7(7) 10 12
O2 Mn2 O3 98.70(14) 11 19_566
O2 Mn2 O3 107.8(6) 9 19_566
O2 Mn2 O3 89.8(5) 10 19_566
O2 Mn2 O3 98.70(14) 12 19_566
O2 Mn2 O3 107.8(5) 11 17_656
O2 Mn2 O3 98.70(14) 9 17_656
O2 Mn2 O3 98.70(14) 10 17_656
O2 Mn2 O3 89.8(5) 12 17_656
O3 Mn2 O3 88.66(4) 19_566 17_656
O2 Mn2 O3 98.70(14) 11 19_666
O2 Mn2 O3 89.8(5) 9 19_666
O2 Mn2 O3 107.8(6) 10 19_666
O2 Mn2 O3 98.70(14) 12 19_666
O3 Mn2 O3 162.4(3) 19_566 19_666
O3 Mn2 O3 88.66(4) 17_656 19_666
O2 Mn2 O3 89.8(5) 11 17_666
O2 Mn2 O3 98.70(14) 9 17_666
O2 Mn2 O3 98.70(14) 10 17_666
O2 Mn2 O3 107.8(5) 12 17_666
O3 Mn2 O3 88.66(4) 19_566 17_666
O3 Mn2 O3 162.4(3) 17_656 17_666
O3 Mn2 O3 88.66(4) 19_666 17_666
O2 Mn2 Ca2 129.7(4) 11 17_556
O2 Mn2 Ca2 129.7(4) 9 17_556
O2 Mn2 Ca2 117.0(4) 10 17_556
O2 Mn2 Ca2 117.0(4) 12 17_556
O3 Mn2 Ca2 48.17(9) 19_566 17_556
O3 Mn2 Ca2 48.17(9) 17_656 17_556
O3 Mn2 Ca2 119.83(11) 19_666 17_556
O3 Mn2 Ca2 119.83(11) 17_666 17_556
O2 Mn2 Ca2 117.0(4) 11 17_666
O2 Mn2 Ca2 117.0(4) 9 17_666
O2 Mn2 Ca2 129.7(4) 10 17_666
O2 Mn2 Ca2 129.7(4) 12 17_666
O3 Mn2 Ca2 119.83(11) 19_566 17_666
O3 Mn2 Ca2 119.83(11) 17_656 17_666
O3 Mn2 Ca2 48.17(9) 19_666 17_666
O3 Mn2 Ca2 48.17(9) 17_666 17_666
Ca2 Mn2 Ca2 112.85(6) 17_556 17_666
O2 Mn2 Ca2 117.0(4) 11 17_566
O2 Mn2 Ca2 129.7(3) 9 17_566
O2 Mn2 Ca2 117.0(4) 10 17_566
O2 Mn2 Ca2 129.7(3) 12 17_566
O3 Mn2 Ca2 48.17(9) 19_566 17_566
O3 Mn2 Ca2 119.83(11) 17_656 17_566
O3 Mn2 Ca2 119.83(11) 19_666 17_566
O3 Mn2 Ca2 48.17(9) 17_666 17_566
Ca2 Mn2 Ca2 72.19(3) 17_556 17_566
Ca2 Mn2 Ca2 72.19(3) 17_666 17_566
O2 Mn2 Ca2 129.7(3) 11 17_656
O2 Mn2 Ca2 117.0(4) 9 17_656
O2 Mn2 Ca2 129.7(3) 10 17_656
O2 Mn2 Ca2 117.0(4) 12 17_656
O3 Mn2 Ca2 119.83(11) 19_566 17_656
O3 Mn2 Ca2 48.17(9) 17_656 17_656
O3 Mn2 Ca2 48.17(9) 19_666 17_656
O3 Mn2 Ca2 119.83(11) 17_666 17_656
Ca2 Mn2 Ca2 72.19(3) 17_556 17_656
Ca2 Mn2 Ca2 72.19(3) 17_666 17_656
Ca2 Mn2 Ca2 112.85(6) 17_566 17_656
O1B Ca1 O1B 54.5(3) 19_566 17_656
O1B Ca1 O1B 54.5(3) 19_566 1_456
O1B Ca1 O1B 80.7(5) 17_656 1_456
O1B Ca1 O1B 80.7(5) 19_566 3_546
O1B Ca1 O1B 54.5(3) 17_656 3_546
O1B Ca1 O1B 54.5(3) 1_456 3_546
O1B Ca1 O1A 11.9(4) 19_566 19_566
O1B Ca1 O1A 62.2(2) 17_656 19_566
O1B Ca1 O1A 62.2(2) 1_456 19_566
O1B Ca1 O1A 92.6(4) 3_546 19_566
O1B Ca1 O1A 62.2(2) 19_566 17_656
O1B Ca1 O1A 11.9(4) 17_656 17_656
O1B Ca1 O1A 92.6(4) 1_456 17_656
O1B Ca1 O1A 62.2(2) 3_546 17_656
O1A Ca1 O1A 68.0(3) 19_566 17_656
O1B Ca1 O1A 92.6(4) 19_566 19_556
O1B Ca1 O1A 62.2(2) 17_656 19_556
O1B Ca1 O1A 62.2(2) 1_456 19_556
O1B Ca1 O1A 11.9(4) 3_546 19_556
O1A Ca1 O1A 104.5(6) 19_566 19_556
O1A Ca1 O1A 68.0(3) 17_656 19_556
O1B Ca1 O1A 62.2(2) 19_566 17_556
O1B Ca1 O1A 92.6(4) 17_656 17_556
O1B Ca1 O1A 11.9(4) 1_456 17_556
O1B Ca1 O1A 62.2(2) 3_546 17_556
O1A Ca1 O1A 68.0(3) 19_566 17_556
O1A Ca1 O1A 104.5(6) 17_656 17_556
O1A Ca1 O1A 68.0(3) 19_556 17_556
O1B Ca1 O2 120.8(3) 19_566 9_445
O1B Ca1 O2 115.8(3) 17_656 9_445
O1B Ca1 O2 66.5(3) 1_456 9_445
O1B Ca1 O2 61.6(3) 3_546 9_445
O1A Ca1 O2 128.2(3) 19_566 9_445
O1A Ca1 O2 121.6(3) 17_656 9_445
O1A Ca1 O2 53.9(3) 19_556 9_445
O1A Ca1 O2 60.3(3) 17_556 9_445
O1B Ca1 O2 115.8(3) 19_566 11_445
O1B Ca1 O2 120.8(3) 17_656 11_445
O1B Ca1 O2 61.6(3) 1_456 11_445
O1B Ca1 O2 66.5(3) 3_546 11_445
O1A Ca1 O2 121.6(3) 19_566 11_445
O1A Ca1 O2 128.2(3) 17_656 11_445
O1A Ca1 O2 60.3(3) 19_556 11_445
O1A Ca1 O2 53.9(3) 17_556 11_445
O2 Ca1 O2 9.6(6) 9_445 11_445
O1B Ca1 O2 66.5(3) 19_566 12
O1B Ca1 O2 61.6(3) 17_656 12
O1B Ca1 O2 120.8(3) 1_456 12
O1B Ca1 O2 115.8(3) 3_546 12
O1A Ca1 O2 60.3(3) 19_566 12
O1A Ca1 O2 53.9(3) 17_656 12
O1A Ca1 O2 121.6(3) 19_556 12
O1A Ca1 O2 128.2(3) 17_556 12
O2 Ca1 O2 170.0(6) 9_445 12
O2 Ca1 O2 177.3(4) 11_445 12
O1B Ca1 O2 61.6(3) 19_566 10
O1B Ca1 O2 66.5(3) 17_656 10
O1B Ca1 O2 115.8(3) 1_456 10
O1B Ca1 O2 120.8(3) 3_546 10
O1A Ca1 O2 53.9(3) 19_566 10
O1A Ca1 O2 60.3(3) 17_656 10
O1A Ca1 O2 128.2(3) 19_556 10
O1A Ca1 O2 121.6(3) 17_556 10
O2 Ca1 O2 177.3(4) 9_445 10
O2 Ca1 O2 170.0(6) 11_445 10
O2 Ca1 O2 9.6(6) 12 10
O3 Ca2 O3 67.63(10) 3_545 1_455
O3 Ca2 O3 103.82(18) 3_545 3
O3 Ca2 O3 67.63(10) 1_455 3
O3 Ca2 O3 67.63(10) 3_545 .
O3 Ca2 O3 103.82(18) 1_455 .
O3 Ca2 O3 67.63(10) 3 .
O3 Ca2 Cl1 138.99(3) 3_545 .
O3 Ca2 Cl1 138.99(3) 1_455 .
O3 Ca2 Cl1 74.44(7) 3 .
O3 Ca2 Cl1 74.44(7) . .
O3 Ca2 Cl1 74.44(7) 3_545 1_445
O3 Ca2 Cl1 74.44(7) 1_455 1_445
O3 Ca2 Cl1 138.99(3) 3 1_445
O3 Ca2 Cl1 138.99(3) . 1_445
Cl1 Ca2 Cl1 133.57(9) . 1_445
O3 Ca2 Cl1 138.99(3) 3_545 1_455
O3 Ca2 Cl1 74.44(7) 1_455 1_455
O3 Ca2 Cl1 74.44(7) 3 1_455
O3 Ca2 Cl1 138.99(3) . 1_455
Cl1 Ca2 Cl1 81.06(3) . 1_455
Cl1 Ca2 Cl1 81.06(3) 1_445 1_455
O3 Ca2 Cl1 74.44(7) 3_545 1_545
O3 Ca2 Cl1 138.99(3) 1_455 1_545
O3 Ca2 Cl1 138.99(3) 3 1_545
O3 Ca2 Cl1 74.44(7) . 1_545
Cl1 Ca2 Cl1 81.06(3) . 1_545
Cl1 Ca2 Cl1 81.06(3) 1_445 1_545
Cl1 Ca2 Cl1 133.57(9) 1_455 1_545
O3 Ca2 Cl1 128.09(9) 3_545 25
O3 Ca2 Cl1 128.09(9) 1_455 25
O3 Ca2 Cl1 128.09(9) 3 25
O3 Ca2 Cl1 128.09(9) . 25
Cl1 Ca2 Cl1 66.78(4) . 25
Cl1 Ca2 Cl1 66.78(4) 1_445 25
Cl1 Ca2 Cl1 66.78(4) 1_455 25
Cl1 Ca2 Cl1 66.78(4) 1_545 25
O3 Ca2 Mn2 36.406(16) 3_545 17_556
O3 Ca2 Mn2 36.406(16) 1_455 17_556
O3 Ca2 Mn2 97.04(8) 3 17_556
O3 Ca2 Mn2 97.04(8) . 17_556
Cl1 Ca2 Mn2 169.64(6) . 17_556
Cl1 Ca2 Mn2 56.79(4) 1_445 17_556
Cl1 Ca2 Mn2 102.59(2) 1_455 17_556
Cl1 Ca2 Mn2 102.59(2) 1_545 17_556
Cl1 Ca2 Mn2 123.58(3) 25 17_556
O3 Ca2 Fe2 36.406(16) 3_545 17_556
O3 Ca2 Fe2 36.406(16) 1_455 17_556
O3 Ca2 Fe2 97.04(8) 3 17_556
O3 Ca2 Fe2 97.04(8) . 17_556
Cl1 Ca2 Fe2 169.64(6) . 17_556
Cl1 Ca2 Fe2 56.79(4) 1_445 17_556
Cl1 Ca2 Fe2 102.59(2) 1_455 17_556
Cl1 Ca2 Fe2 102.59(2) 1_545 17_556
Cl1 Ca2 Fe2 123.58(3) 25 17_556
Mn2 Ca2 Fe2 0.00(3) 17_556 17_556
O3 Ca2 Fe2 97.04(8) 3_545 17_666
O3 Ca2 Fe2 97.04(8) 1_455 17_666
O3 Ca2 Fe2 36.406(16) 3 17_666
O3 Ca2 Fe2 36.406(16) . 17_666
Cl1 Ca2 Fe2 56.79(4) . 17_666
Cl1 Ca2 Fe2 169.64(6) 1_445 17_666
Cl1 Ca2 Fe2 102.59(2) 1_455 17_666
Cl1 Ca2 Fe2 102.59(2) 1_545 17_666
Cl1 Ca2 Fe2 123.58(3) 25 17_666
Mn2 Ca2 Fe2 112.85(6) 17_556 17_666
Fe2 Ca2 Fe2 112.85(6) 17_556 17_666
Ca2 Cl1 Ca2 133.57(9) . 1_665
Ca2 Cl1 Ca2 81.06(3) . 1_655
Ca2 Cl1 Ca2 81.06(3) 1_665 1_655
Ca2 Cl1 Ca2 81.06(3) . 1_565
Ca2 Cl1 Ca2 81.06(3) 1_665 1_565
Ca2 Cl1 Ca2 133.57(9) 1_655 1_565
Ca2 Cl1 Ca2 113.22(4) . 25
Ca2 Cl1 Ca2 113.22(4) 1_665 25
Ca2 Cl1 Ca2 113.22(4) 1_655 25
Ca2 Cl1 Ca2 113.22(4) 1_565 25
O1B O1A O1B 90(3) 17_655 .
O1B O1A O1A 44.9(16) 17_655 17_655
O1B O1A O1A 44.9(16) . 17_655
O1B O1A Fe1 82.6(5) 17_655 1_545
O1B O1A Fe1 82.6(5) . 1_545
O1A O1A Fe1 79.5(4) 17_655 1_545
O1B O1A Mn1 82.6(5) 17_655 1_545
O1B O1A Mn1 82.6(5) . 1_545
O1A O1A Mn1 79.5(4) 17_655 1_545
Fe1 O1A Mn1 0.0 1_545 1_545
O1B O1A Mn1 82.6(5) 17_655 .
O1B O1A Mn1 82.6(5) . .
O1A O1A Mn1 79.5(4) 17_655 .
Fe1 O1A Mn1 159.0(9) 1_545 .
Mn1 O1A Mn1 159.0(9) 1_545 .
O1B O1A Fe1 82.6(5) 17_655 .
O1B O1A Fe1 82.6(5) . .
O1A O1A Fe1 79.5(4) 17_655 .
Fe1 O1A Fe1 159.0(9) 1_545 .
Mn1 O1A Fe1 159.0(9) 1_545 .
Mn1 O1A Fe1 0.0 . .
O1B O1A Ca1 172.7(18) 17_655 17_656
O1B O1A Ca1 82.8(14) . 17_656
O1A O1A Ca1 127.7(3) 17_655 17_656
Fe1 O1A Ca1 96.4(2) 1_545 17_656
Mn1 O1A Ca1 96.4(2) 1_545 17_656
Mn1 O1A Ca1 96.4(2) . 17_656
Fe1 O1A Ca1 96.4(2) . 17_656
O1B O1A Ca1 82.8(14) 17_655 17_556
O1B O1A Ca1 172.7(18) . 17_556
O1A O1A Ca1 127.7(3) 17_655 17_556
Fe1 O1A Ca1 96.4(2) 1_545 17_556
Mn1 O1A Ca1 96.4(2) 1_545 17_556
Mn1 O1A Ca1 96.4(2) . 17_556
Fe1 O1A Ca1 96.4(2) . 17_556
Ca1 O1A Ca1 104.5(6) 17_656 17_556
O1B O1A Ca1 3.8(14) 17_655 1_554
O1B O1A Ca1 86.1(18) . 1_554
O1A O1A Ca1 41.1(2) 17_655 1_554
Fe1 O1A Ca1 82.1(4) 1_545 1_554
Mn1 O1A Ca1 82.1(4) 1_545 1_554
Mn1 O1A Ca1 82.1(4) . 1_554
Fe1 O1A Ca1 82.1(4) . 1_554
Ca1 O1A Ca1 168.9(5) 17_656 1_554
Ca1 O1A Ca1 86.62(11) 17_556 1_554
O1B O1A Ca1 86.1(18) 17_655 1_654
O1B O1A Ca1 3.8(14) . 1_654
O1A O1A Ca1 41.1(2) 17_655 1_654
Fe1 O1A Ca1 82.1(4) 1_545 1_654
Mn1 O1A Ca1 82.1(4) 1_545 1_654
Mn1 O1A Ca1 82.1(4) . 1_654
Fe1 O1A Ca1 82.1(4) . 1_654
Ca1 O1A Ca1 86.62(11) 17_656 1_654
Ca1 O1A Ca1 168.9(5) 17_556 1_654
Ca1 O1A Ca1 82.2(4) 1_554 1_654
O1A O1B O1A 90(3) 17_655 .
O1A O1B O1B 45.1(16) 17_655 17_655
O1A O1B O1B 45.1(16) . 17_655
O1A O1B Fe1 82.6(4) 17_655 1_545
O1A O1B Fe1 82.6(4) . 1_545
O1B O1B Fe1 79.5(4) 17_655 1_545
O1A O1B Mn1 82.6(4) 17_655 1_545
O1A O1B Mn1 82.6(4) . 1_545
O1B O1B Mn1 79.5(4) 17_655 1_545
Fe1 O1B Mn1 0.0 1_545 1_545
O1A O1B Fe1 82.6(4) 17_655 .
O1A O1B Fe1 82.6(4) . .
O1B O1B Fe1 79.5(4) 17_655 .
Fe1 O1B Fe1 159.0(7) 1_545 .
Mn1 O1B Fe1 159.0(7) 1_545 .
O1A O1B Mn1 82.6(4) 17_655 .
O1A O1B Mn1 82.6(4) . .
O1B O1B Mn1 79.5(4) 17_655 .
Fe1 O1B Mn1 159.0(7) 1_545 .
Mn1 O1B Mn1 159.0(7) 1_545 .
Fe1 O1B Mn1 0.0 . .
O1A O1B Ca1 175.4(17) 17_655 17_656
O1A O1B Ca1 85.3(15) . 17_656
O1B O1B Ca1 130.3(2) 17_655 17_656
Fe1 O1B Ca1 96.8(2) 1_545 17_656
Mn1 O1B Ca1 96.8(2) 1_545 17_656
Fe1 O1B Ca1 96.8(2) . 17_656
Mn1 O1B Ca1 96.8(2) . 17_656
O1A O1B Ca1 85.3(15) 17_655 1_654
O1A O1B Ca1 175.4(17) . 1_654
O1B O1B Ca1 130.3(2) 17_655 1_654
Fe1 O1B Ca1 96.8(2) 1_545 1_654
Mn1 O1B Ca1 96.8(2) 1_545 1_654
Fe1 O1B Ca1 96.8(2) . 1_654
Mn1 O1B Ca1 96.8(2) . 1_654
Ca1 O1B Ca1 99.3(4) 17_656 1_654
O1A O1B Ca1 6.1(15) 17_655 1_554
O1A O1B Ca1 84.1(17) . 1_554
O1B O1B Ca1 39.00(15) 17_655 1_554
Fe1 O1B Ca1 81.9(3) 1_545 1_554
Mn1 O1B Ca1 81.9(3) 1_545 1_554
Fe1 O1B Ca1 81.9(3) . 1_554
Mn1 O1B Ca1 81.9(3) . 1_554
Ca1 O1B Ca1 169.3(4) 17_656 1_554
Ca1 O1B Ca1 91.33(10) 1_654 1_554
O1A O1B Ca1 84.1(17) 17_655 17_556
O1A O1B Ca1 6.1(15) . 17_556
O1B O1B Ca1 39.00(15) 17_655 17_556
Fe1 O1B Ca1 81.9(3) 1_545 17_556
Mn1 O1B Ca1 81.9(3) 1_545 17_556
Fe1 O1B Ca1 81.9(3) . 17_556
Mn1 O1B Ca1 81.9(3) . 17_556
Ca1 O1B Ca1 91.33(10) 17_656 17_556
Ca1 O1B Ca1 169.3(4) 1_654 17_556
Ca1 O1B Ca1 78.0(3) 1_554 17_556
O2 O2 Fe2 81.0(5) 2 9_444
O2 O2 Mn2 81.0(5) 2 9_444
Fe2 O2 Mn2 0.0 9_444 9_444
O2 O2 Mn1 81.1(5) 2 9_445
Fe2 O2 Mn1 162.1(10) 9_444 9_445
Mn2 O2 Mn1 162.1(10) 9_444 9_445
O2 O2 Fe1 81.1(5) 2 9_445
Fe2 O2 Fe1 162.1(10) 9_444 9_445
Mn2 O2 Fe1 162.1(10) 9_444 9_445
Mn1 O2 Fe1 0.0 9_445 9_445
O2 O2 Ca1 130.2(3) 2 9_554
Fe2 O2 Ca1 97.1(4) 9_444 9_554
Mn2 O2 Ca1 97.1(4) 9_444 9_554
Mn1 O2 Ca1 94.4(4) 9_445 9_554
Fe1 O2 Ca1 94.4(4) 9_445 9_554
O2 O2 Ca1 130.2(3) 2 9_544
Fe2 O2 Ca1 97.1(4) 9_444 9_544
Mn2 O2 Ca1 97.1(4) 9_444 9_544
Mn1 O2 Ca1 94.4(4) 9_445 9_544
Fe1 O2 Ca1 94.4(4) 9_445 9_544
Ca1 O2 Ca1 99.6(6) 9_554 9_544
O2 O2 Ca1 40.9(2) 2 9_444
Fe2 O2 Ca1 84.4(4) 9_444 9_444
Mn2 O2 Ca1 84.4(4) 9_444 9_444
Mn1 O2 Ca1 82.1(4) 9_445 9_444
Fe1 O2 Ca1 82.1(4) 9_445 9_444
Ca1 O2 Ca1 170.7(5) 9_554 9_444
Ca1 O2 Ca1 89.28(8) 9_544 9_444
O2 O2 Ca1 40.9(2) 2 9_454
Fe2 O2 Ca1 84.4(4) 9_444 9_454
Mn2 O2 Ca1 84.4(4) 9_444 9_454
Mn1 O2 Ca1 82.1(4) 9_445 9_454
Fe1 O2 Ca1 82.1(4) 9_445 9_454
Ca1 O2 Ca1 89.28(8) 9_554 9_454
Ca1 O2 Ca1 170.7(5) 9_544 9_454
Ca1 O2 Ca1 81.7(4) 9_444 9_454
Fe2 O3 Mn2 0.00(6) 17_656 17_656
Fe2 O3 Fe2 162.4(3) 17_656 17_666
Mn2 O3 Fe2 162.4(3) 17_656 17_666
Fe2 O3 Mn2 162.4(3) 17_656 17_666
Mn2 O3 Mn2 162.4(3) 17_656 17_666
Fe2 O3 Mn2 0.00(6) 17_666 17_666
Fe2 O3 Ca2 95.42(8) 17_656 1_655
Mn2 O3 Ca2 95.42(8) 17_656 1_655
Fe2 O3 Ca2 95.42(8) 17_666 1_655
Mn2 O3 Ca2 95.42(8) 17_666 1_655
Fe2 O3 Ca2 95.42(8) 17_656 .
Mn2 O3 Ca2 95.42(8) 17_656 .
Fe2 O3 Ca2 95.42(8) 17_666 .
Mn2 O3 Ca2 95.42(8) 17_666 .
Ca2 O3 Ca2 103.82(18) 1_655 .
Fe2 O3 Ca1 83.32(11) 17_656 17_556
Mn2 O3 Ca1 83.32(11) 17_656 17_556
Fe2 O3 Ca1 83.32(11) 17_666 17_556
Mn2 O3 Ca1 83.32(11) 17_666 17_556
Ca2 O3 Ca1 168.64(15) 1_655 17_556
Ca2 O3 Ca1 87.54(5) . 17_556
Fe2 O3 Ca1 83.32(11) 17_656 17_656
Mn2 O3 Ca1 83.32(11) 17_656 17_656
Fe2 O3 Ca1 83.32(11) 17_666 17_656
Mn2 O3 Ca1 83.32(11) 17_666 17_656
Ca2 O3 Ca1 87.54(5) 1_655 17_656
Ca2 O3 Ca1 168.64(15) . 17_656
Ca1 O3 Ca1 81.10(13) 17_556 17_656
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mn1 O2 1.904(8) 10_554
Mn1 O2 1.904(8) 28
Mn1 O2 1.904(8) 12_554
Mn1 O2 1.904(8) 26
Mn1 O2 1.904(8) 25
Mn1 O2 1.904(8) 27
Mn1 O2 1.904(8) 11_554
Mn1 O2 1.904(8) 9_554
Mn1 O1B 1.930(2) 19_565
Mn1 O1B 1.930(2) 3_655
Mn1 O1B 1.930(2) 17_655
Mn1 O1B 1.930(2) 1_565
Fe1 O2 1.904(8) 10_554
Fe1 O2 1.904(8) 28
Fe1 O2 1.904(8) 12_554
Fe1 O2 1.904(8) 26
Fe1 O2 1.904(8) 25
Fe1 O2 1.904(8) 27
Fe1 O2 1.904(8) 11_554
Fe1 O2 1.904(8) 9_554
Fe1 O1B 1.930(2) 19_565
Fe1 O1B 1.930(2) 3_655
Fe1 O1B 1.930(2) 17_655
Fe1 O1B 1.930(2) 1_565
Mn2 O2 1.888(8) 11
Mn2 O2 1.888(8) 9
Mn2 O2 1.888(8) 10
Mn2 O2 1.888(8) 12
Mn2 O3 1.9207(8) 19_566
Mn2 O3 1.9207(8) 17_656
Mn2 O3 1.9207(8) 19_666
Mn2 O3 1.9207(8) 17_666
Mn2 Ca2 3.2217(11) 17_556
Mn2 Ca2 3.2217(11) 17_666
Mn2 Ca2 3.2217(11) 17_566
Mn2 Ca2 3.2217(11) 17_656
Ca1 O1B 2.390(8) 19_566
Ca1 O1B 2.390(8) 17_656
Ca1 O1B 2.390(8) 1_456
Ca1 O1B 2.390(8) 3_546
Ca1 O1A 2.400(9) 19_566
Ca1 O1A 2.400(9) 17_656
Ca1 O1A 2.400(9) 19_556
Ca1 O1A 2.400(9) 17_556
Ca1 O2 2.485(12) 9_445
Ca1 O2 2.485(12) 11_445
Ca1 O2 2.485(12) 12
Ca1 O2 2.485(12) 10
Ca2 O3 2.412(3) 3_545
Ca2 O3 2.412(3) 1_455
Ca2 O3 2.412(3) 3
Ca2 O3 2.412(3) .
Ca2 Cl1 2.9207(10) .
Ca2 Cl1 2.9207(10) 1_445
Ca2 Cl1 2.9207(10) 1_455
Ca2 Cl1 2.9207(10) 1_545
Ca2 Cl1 3.216(2) 25
Ca2 Mn2 3.2217(11) 17_556
Ca2 Fe2 3.2217(11) 17_556
Ca2 Fe2 3.2217(11) 17_666
Cl1 Ca2 2.9207(10) 1_665
Cl1 Ca2 2.9207(10) 1_655
Cl1 Ca2 2.9207(10) 1_565
Cl1 Ca2 3.216(2) 25
O1A O1B 0.498(14) 17_655
O1A O1B 0.498(14) .
O1A O1A 0.70(3) 17_655
O1A Fe1 1.930(3) 1_545
O1A Mn1 1.930(3) 1_545
O1A Ca1 2.400(9) 17_656
O1A Ca1 2.400(9) 17_556
O1A Ca1 2.886(12) 1_554
O1A Ca1 2.886(12) 1_654
O1B O1A 0.498(14) 17_655
O1B O1B 0.70(2) 17_655
O1B Fe1 1.930(2) 1_545
O1B Mn1 1.930(2) 1_545
O1B Ca1 2.390(8) 17_656
O1B Ca1 2.390(8) 1_654
O1B Ca1 2.895(10) 1_554
O1B Ca1 2.895(10) 17_556
O2 O2 0.59(3) 2
O2 Fe2 1.888(8) 9_444
O2 Mn2 1.888(8) 9_444
O2 Mn1 1.904(8) 9_445
O2 Fe1 1.904(8) 9_445
O2 Ca1 2.485(11) 9_554
O2 Ca1 2.485(11) 9_544
O2 Ca1 2.901(13) 9_444
O2 Ca1 2.901(13) 9_454
O3 Fe2 1.9207(8) 17_656
O3 Mn2 1.9207(8) 17_656
O3 Fe2 1.9207(8) 17_666
O3 Mn2 1.9207(8) 17_666
O3 Ca2 2.412(3) 1_655
O3 Ca1 2.920(4) 17_556
O3 Ca1 2.920(4) 17_656
